$K and continuous to grow up to $S_m =0.8 * (2RLn4)$ at T = 40K. Similar behavior is observed in the $x=1$ sample (i.e. Ce$_2$Ni$_2$Sn) but with $S_(T)$ increasing in a more monotonous manner. Compared with the $S_m(T)$ behavior of a sharp energy distribution of levels, provided by the results depicted in Fig. \[F5\]a, it becomes evident an overlap of the side levels of the ground and first excited CFE levels.

This is the key to understand the complex magnetic behavior of this Ni-rich alloys which show a decrease of the magnetic moment with a simultaneous increase of a weak $T_{N2}$. The former effect is driven by the increase of the $4f$ state hybridization whereas the latter is driven by the increase of the GS density of states due to the arising contribution of the low energy levels of the CFE excited state. Such an enhancement of the low energy density of states is supported by the increasing $C_m/T$ contribution to the specific heat above $T_{N2}$ deduced from Fig. \[F6\], which increases from 0.2J/molK$^2$ for x = 0.5 up to 0.45J/molK$^2$ for x=1 around $T\approx 15$K. Low effective moments and relatively high ordering temperatures are typical of itinerant magnetic systems [@DeLong], provided that the density of states is large enough. This scenario is favored by the reduction of the Ce-Ce spacings decrease driven by the reduction of $a$ and $b$ lattice parameters.

Within a simplified picture, such would be the expected way to undergo from a N = 2 degenerated GS to a N = 4 degenerated GS in a continuous way. In Fig. \[F5\]b we include a theoretical prediction [@Coqblin] for a N=4 degenerated state with a characteristic temperature $T_o=30$K. This comparison clearly indicates that, despite of the energy levels contribution of the first excited CFE state, the N=4 GS is not reached in this system. Similar situation was observed in other strongly anisotropic Ce systems such as CeTiGe [@Micha].

The low temperature magnetic properties are resumed in the magnetic phase diagram presented in Fig. \[F7\]. On the Pd-rich
$ K and continuous to grow up to $ S_m = 0.8 * (2RLn4)$ at T = 40K. Similar demeanor is observe in the $ x=1 $ sample (i.e. Ce$_2$Ni$_2$Sn) but with $ S_(T)$ increase in a more flat manner. Compared with the $ S_m(T)$ behavior of a astute department of energy distribution of levels, provided by the results depicted in Fig.   \[F5\]a, it becomes discernible an overlap of the side horizontal surface of the flat coat and first excited CFE levels. 

 This is the key to understand the complex charismatic behavior of this Ni - rich alloys which testify a decrease of the magnetic moment with a coincident increase of a watery $ T_{N2}$. The former effect is driven by the increase of the $ 4f$ state hybridization whereas the latter is drive by the increase of the GS density of states due to the arising contribution of the low department of energy degree of the CFE excited state. Such an enhancement of the low energy density of states is supported by the increasing $ C_m / T$ contribution to the specific heat above $ T_{N2}$ deduce from Fig.   \[F6\ ], which increases from 0.2J / molK$^2 $ for x = 0.5 up to 0.45J / molK$^2 $ for x=1 around $ T\approx 15$K. Low effective here and now and relatively gamey ordering temperatures are distinctive of itinerant magnetic system [ @DeLong ], provided that the density of country is large enough. This scenario is favored by the reduction of the Ce - Ce spacings decrease driven by the reduction of $ a$ and $ b$ wicket parameters. 

 Within a simplified picture, such would be the expected way to undergo from a N = 2 degenerated GS to a N = 4 degenerated GS in a continuous way. In Fig.   \[F5\]b we admit a theoretical prediction [ @Coqblin ] for a N=4 degenerated department of state with a characteristic temperature $ T_o=30$K. This comparison clearly indicates that, despite of the energy levels contribution of the inaugural excited CFE state, the N=4 GS is not reached in this arrangement. Similar situation was observed in other powerfully anisotropic Ce systems such as CeTiGe [ @Micha ]. 

 The low temperature magnetic properties are resumed in the charismatic phase diagram presented in Fig.   \[F7\ ]. On the Pd - rich
$K ajd continuous to grow up to $S_m =0.8 * (2RLn4)$ at T = 40K. Smmilar gehavior is observed in the $x=1$ sample (i.w. Ce$_2$Nu$_2$Sn) but with $S_(T)$ increaring in a more mobotoious manner. Compeded witm the $D_m(T)$ yeiavior of a shatp energy divtribution of nexeps, provided by the results depicted in Fig. \[G5\]a, it becomes evydenu ag ovsglcp of the side levels of the grkund anv first excited CFE levels.

This is the key to knderstand the comolex magnetuc bqyavior of thks Ni-rich alloys which show a decrease of the magnetiz momznt with a winulhdneous incrxase os a weak $T_{N2}$. Bne forker effrct is driven ny thx inxrease of the $4f$ state hybridization wheteas the ldtcer is driven by the unxreasg of dhe EW ddnsjtb or statfs vue to the zrising conrribution of the loe qbergy levels kf the CSE excited state. Such an enhancement of ths low energy density of states is supported hy the insreasing $C_m/T$ contribution to the specific heat abmve $T_{I2}$ aedbgcd ffim Fig. \[F6\], which increases from 0.2J/molK$^2$ for x = 0.5 up tj 0.45J/kokK$^2$ for x=1 arounb $T\approx 15$K. Low rfvevjive moments avd relcfibely high ordering temperwturew are typycal of itinerant magnetic systwms [@DeLong], pgovieed that the densicy of states is karge enough. This scenario ir fabored by thf reductikv of the Ce-Ce spxcikgs decreast driven by the requction oh $a$ aud $b$ latgice paramqters.

Withij a slkplified picture, skch wlund be the fxpected way to undergo from a I = 2 degeneratgd CS no a N = 4 begenevated GS in a cjntinuous way. Nn Fig. \[F5\]b we ivclude a tgeoretiral predictijn [@Coqblin] fos a N=4 degenereted statq wirh a characgdristic tempersture $T_o=30$K. This compqrison clearly indlcater that, despite oy uhw energy levelx cuntwihuvion jx the first axciged VFE sgate, tht N=4 ES ix not reached in thiv syatem. Similar situayijn was ovserved yn other stromgly anisotropic Ct systxms surh as VeTyGe [@Micha].

The low temperature mzgnetic pgopcrties are refumee in the maguetic phase diagram presented in Fig. \[F7\]. On the Pd-rich
$K and continuous to grow up to * at T 40K. Similar behavior sample Ce$_2$Ni$_2$Sn) but with increasing in a monotonous manner. Compared with the $S_m(T)$ of a sharp energy distribution of levels, provided by the results depicted in \[F5\]a, it becomes evident an overlap of the side levels of the ground first CFE This the key to understand the complex magnetic behavior of this Ni-rich alloys which show a decrease the magnetic moment with a simultaneous increase of weak $T_{N2}$. The former is driven by the increase the state hybridization the is by the increase the GS density of states due to the arising contribution of the low energy levels of the excited state. enhancement of low density states is supported increasing $C_m/T$ contribution to the specific deduced from Fig. \[F6\], which increases from 0.2J/molK$^2$ x = up to 0.45J/molK$^2$ for x=1 around 15$K. Low effective moments and relatively high ordering are typical of itinerant magnetic systems [@DeLong], provided that the density of states is large scenario is favored by reduction of the spacings driven the of $a$ $b$ lattice parameters. Within a simplified picture, such would be the way to undergo from a N = 2 degenerated GS N 4 degenerated GS a continuous way. In \[F5\]b include a theoretical prediction a degenerated characteristic $T_o=30$K. comparison clearly indicates that, of the energy levels contribution the first excited CFE not reached in this system. Similar situation was in other strongly anisotropic Ce systems such CeTiGe [@Micha]. The low temperature magnetic properties are resumed in the magnetic diagram presented \[F7\]. On the Pd-rich
$K and continuous to grow up to $S_M =0.8 * (2RLn4)$ at T = 40K. SiMilar BehAviOr Is obServEd in the $x=1$ sample (I.E. Ce$_2$NI$_2$Sn) but with $S_(T)$ increasing In a moRe MOnotONoUs manNer. CompAReD WIth ThE $S_M(T)$ bEhAViOr of a ShaRp energY distributIon Of Levels, providED bY the resultS dePicted in Fig. \[F5\]A, it BecomeS eVidENt an oVerLap of The sidE Levels Of the grouNd ANd firsT Excited cfe lEvelS.

This is the key to unDErSTand the complex MagnetIc BEhAVIor Of tHis Ni-rich aLlOys whICh show a DEcREASe oF The magnetic moMent with a siMUltAneous InCreASe of a wEak $T_{N2}$. thE ForMer effect is DrivEn by the inCrease OF the $4f$ stATe hybriDizatiOn wHerEas tHE lAtTer Is DRivEN bY thE IncRease of tHe gS DensiTy of STATEs duE to The aRisinG contribution Of tHe loW EneRgy leVels oF the cFe exciTed staTe. SucH aN enhancement of tHe loW energy deNsiTy Of sTaTes is SUpportEd bY thE increaSing $C_m/T$ COntRiBUTIoN to the specific heat AbOVE $T_{n2}$ deduced From FiG. \[f6\], wHiCH increasEs FroM 0.2J/moLk$^2$ For x = 0.5 uP to 0.45J/MOlk$^2$ for x=1 aroUnd $T\apPRoX 15$K. low effeCtIve momEnTs aNd rElatiVEly hIgh ordEring temPeratURes are typical oF Itinerant magnETiC SYsTEms [@DELoNg], provided tHat tHE denSity OF sTatES is laRge enOuGH. THIs scenario is favored By The redUctioN of the Ce-Ce spaCings decreASE Driven by The rEDuCTion of $a$ and $b$ latTice pArameters.

WIThin a simPlifiEd picturE, such woulD BE the expeCteD waY to UndERGo From a N = 2 degenerATEd GS To A N = 4 degenEraTed GS in A coNtiNuoUs wAy. in Fig. \[F5\]b we Include a ThEoReTiCal PrediCTion [@CoqbLiN] foR a n=4 deGenerATed staTe witH a chArAcTEriStic temPErATUre $T_O=30$K. thIs coMpaRiSon clEarlY IndIcates tHat, despitE of THe enErGy Levels cOntribution of ThE first exciTeD CFe state, THE N=4 GS is noT reached in this system. SimILar situAtiOn was ObseRved in othEr sTronglY anISotropIc Ce syStems SuCh aS cETiGe [@mIChA].

ThE lOw temperatURE maGnetiC pRopeRties arE resumed in the magneTIc pHase diagram prEseNted IN fiG. \[F7\]. ON ThE pd-rIcH
$K and continuous to growup to $S_m  =0.8  *(2R Ln 4)$at T  = 40K. Simila r  beh avior is observed in t he $x =1 $  sam p le  (i.e . Ce$_2 $ Ni $ _ 2$S n)  b utwi t h$S_(T )$increas ing in a m ore  m onotonous ma n ne r. Compare d w ith the $S_m (T) $ beha vi oro f a s har p ene rgy di s tribut ion of le ve l s, pro v ided by t he  res ults depicted inF ig .  \[F5\]a, it b ecomes  e v id e n t a n o verlap ofth e sid e  levels of t h e g r ound and firs t excited C F E l evels. 
Thi s  is th e key  t o  un derstand th e co mplex mag neticb ehavior of this  Ni-ri chall oysw hi ch  sh ow a d e cr eas e  of  the mag ne ti c mom entw i t h  a s imu ltan eousincrease of a  we ak $ T _{N 2}$.The f orme reffec t is d riven  b y the increaseof t he $4f$ s tat ehyb ri dizat i on whe rea s t he latt er is d r ive nb y th e increase of theGS d en sity ofstates du et o the ar is ing  con t r ibuti on o f  t he low e nergyl ev el s of th eCFE ex ci ted  st ate.S uchan enh ancement  of t h e low energy d e nsity of stat e si s  s u ppor ted  by the inc reas i ng $ C_m/ T $con t ribut ion t ot he specific heat above  $ T_{N2} $ ded uced from Fig . \[F6\],w h i ch incre ases fr o m 0.2J/molK$^2 $ for  x = 0.5 u p  to 0.45 J/mol K$^2$ fo r x=1 aro u n d $T\app rox  15 $K.  Lo w ef fective momen t s  and  r elative lyhigh or der ing  te mpe ra tures are  typical  o fit in era nt ma g netic sy st ems  [ @De Long] ,  provi ded t hatth ed ens ity ofs ta t e s is  l ar ge e nou gh . Thi s sc e nar io is f avored by  th e  red uc ti on of t he Ce-Ce spac in gs decreas edri ven by t he reduc tion of $a$ and $b$ lat t ice par ame ters. 

Wi thin a si mpl ifiedpic t ure, s uch wo uld b ethe e xpect e d  w ayto  undergo f r o m a  N =2dege nerated  GS to a N = 4 deg e ner ated GS in acon tinu o u sway .  I n  Fi g. \[F 5 \ ]b we include a  theoretic al pr ediction [ @ Coq bl in] for  a N=4degen e rated s tate with  a charac te rist i c  te mperature$T_o=30$ K. This c o mpari s on  clea rly  indic at esthat,  despi t e o f the  energ ylevels  cont ri bution o f the first excited CFE  state , the  N= 4 GS is n otr eac hed in th is s ystem. Sim ila r s ituat ion was o bser v ed  in other  str o ngly anis o tr opi c Ce  systems su c h asCeTiG e [ @ Micha] .

T he low temperatur e  magnetic prop erti e s  ar e r e sume din the magneti c p ha s e  diagram  p resented in  Fig. \[ F7 \ ]. On  the P d-rich 
$K and_continuous to_grow up to $S_m_=0.8 *_(2RLn4)$_at T_=_40K. Similar behavior_is observed in_the $x=1$ sample (i.e._Ce$_2$Ni$_2$Sn) but with_$S_(T)$_increasing in a more monotonous manner. Compared with the $S_m(T)$ behavior of a sharp_energy_distribution of_levels,_provided_by the results depicted in_Fig. \[F5\]a, it becomes evident an_overlap of_the side levels of the ground and first_excited_CFE levels.

This is_the key to understand the complex magnetic behavior of_this Ni-rich alloys which show a_decrease of the_magnetic_moment_with a simultaneous increase_of a weak $T_{N2}$. The former_effect is driven by the increase_of the $4f$ state hybridization whereas the_latter is driven by the increase_of the GS density of_states due_to the arising contribution of_the low energy_levels of_the CFE excited_state. Such an enhancement of the_low energy density_of states is supported by the_increasing_$C_m/T$ contribution to_the_specific_heat above_$T_{N2}$ deduced from_Fig. \[F6\],_which increases_from_0.2J/molK$^2$ for x = 0.5 up_to_0.45J/molK$^2$ for x=1 around $T\approx 15$K. Low_effective moments and relatively_high_ordering temperatures are typical_of itinerant magnetic systems [@DeLong],_provided that the density of states_is large_enough. This_scenario is favored by the reduction of the Ce-Ce spacings decrease_driven by the reduction of $a$_and $b$ lattice parameters.

Within_a simplified_picture,_such would be_the_expected way_to undergo from a N = 2_degenerated GS_to a N = 4 degenerated_GS in a continuous_way._In Fig. \[F5\]b we include a theoretical_prediction [@Coqblin] for a N=4 degenerated_state with a characteristic temperature_$T_o=30$K._This_comparison clearly indicates that, despite_of the energy levels contribution of_the first excited_CFE state, the N=4 GS is not_reached_in this system. Similar situation was_observed_in other strongly anisotropic Ce systems_such_as_CeTiGe [@Micha].

The low temperature magnetic_properties are resumed in the magnetic_phase diagram presented in Fig. \[F7\]. On the Pd-rich